Quality and high yield synthesis of Ag nanowires by microwave-assisted hydrothermal method
© Meléndrez et al.; licensee Springer. 2015
Received: 16 December 2014
Accepted: 20 January 2015
Published: 6 February 2015
Silver nanowires (Ag-NWs) were obtained using microwave-assisted hydrothermal method (MAH). The main advantage of the method is its high NWs production which is greater than 90%. It is also easy, fast, and highly reproducible process. One of the drawbacks presented so far in the synthesis of nanostructures by polyol path is the high temperature used in the process, which is superior than the boiling point of solvent (ethylene glycol), and also its excessive reaction time. Here, Ag-NWs with diameters of 70 to 110 nm were synthesized in 5 min in large quantities. Results showed that dimensions and shape of nanowires were very susceptible to changes with reaction parameters. The reactor power and reactor fill capacity were important for the synthesis. It was found that the reaction time needs to be decreased because of the NWs which start to deform and break up due to significant increase in the pressure's system. Energy-dispersive X-ray spectroscopy and electron diffraction analysis (SAED) did not show corresponding phases of AgO. Some aspects about synthesis parameters which are related to the percent yield and size of nanowires are also discussed.
KeywordsNanowires Hydrothermal synthesis Nanostructures Microwave
One-dimensional (1D) silver nanowires (Ag-NWs) are among the most important nanomaterials due to their potential applications in photoluminescence , photonic crystals , surface-enhanced Raman scattering , isotropic conductive adhesives , field emission devices , high-density magnetic recording devices , and sensors . It functions mainly as interconnects or active components in fabricating nanodevices. Control of appropriate shape and size of Ag-NWs can be used efficiently in the diverse applications as mentioned above. Efforts have currently been focused in the control of the synthesis process and assembly of such nanostructures. For this reason, it is important to understand its synthesis process. It has been found that Ag-NWs have exceptional thermal, electrical, and optical properties. Transparent conductive films of Ag-NWs have demonstrated potential to replace indium tin oxide (ITO) in solar cells, displays, touch panels, and organic light-emitting diodes (OLED) .
There are many physical [9-15] and chemical [16-20] methods that have been reported for synthesizing Ag-NWs. The percentage yield of the nanowires is an important factor. In most of these processes, nanoparticles and mixtures of other nanostructures are hard to deal with their separation; therefore they limit their use due to different sizes. The use of precursor molecules of preferential growth, like cetyl trimethylammonium bromide (CTAB) or polyvinylpyrrolidone (PVP) sometimes also significantly have proved disadvantageous as they interact strongly with the metal surface, increasing the reaction times and requiring higher temperatures. Moreover, the use of template synthesis to control the diameter and morphology  also proves that it is complicated.
Reduction of AgNO3 in ethylene glycol, known as polyol method, is the most widely used chemical method to synthesize Ag-NWs, where PVP is used as the precursor molecule of preferential growth. Xia et al.  and Sun et al.  improved this method and obtained Ag-NWs with high aspect ratios at a well-defined reactant addition rate in a dried ethylene glycol system. Low precursor concentrations and a slow addition in the reaction medium forms multiply twinned particles (MTPs) just when the nucleation process starts, and these particles serve as seeds to grow silver nanowires .
High-purity, uniform, and smaller Ag-NWs can also be obtained from the modified polyol method which also increases the yield percentage. Adding redox active metal salts like (FeII/FeIII or CuI/CuII) [25,26], Na2S , and NaCl  or introducing Pt seeds in the presence of PVP  facilitates a controlled growth of nanowires. This occurs because of the NWs which are grown from multiple-twinned seeds with a decahedral structure, while seeds with a single-crystal structure tend to evolve into polyhedral nanocrystals with a cubic or octahedral shape. Therefore, for producing high yield, it becomes a necessity to develop an efficient way to promote the formation of multiple-twinned seeds at the nucleation stage during the synthesis . Investigations on synthesis mechanism elucidates that these variable valency metal ions having low valence can remove oxygen from the solvent preventing twinned seeds that are dissolved by oxidative etching during the initial formation of seeds, thereby scavenging absorbed atomic oxygen from the surface of seeds. For this reason, the formation of AgCl colloid results in slow releasing of Ag+ in the solution, which facilitates the formation of Ag-NWs . However, it is important to mention other works that have been focused on improving the size, controlling the shape, increasing the yield percentage, and reproducibility of the reaction to obtain high-purity silver nanowires that are still ongoing as there has not been found an efficient method.
In this work, we report a microwave-assisted hydrothermal method where microwaves directly heats the volume of liquid while the environment or the containers are heated only by reaction's mixture, in order to achieve high-quality and yield Ag-NWs. As molecules with dipolar structure (e.g., ethylene glycol, PVP) oscillate in a microwave fluctuating field, this oscillation generates a molecular movement resulting in friction leading to heat. Another advantage is that molecules having an ionic structure (e.g., AgNO3) get aligned in the electromagnetic field facilitating a favorable nucleation and growth processes of the 1D nanostructures. This method significantly reduces reaction time compared to the conventional heating time, whereby yielding high-quality, narrow size good-shaped Ag-NWs, and reproducibility is very high in this method.
Ag-NWs were synthesized by microwave-assisted hydrothermal method (MAH). In this process, silver nitrate (AgNO3), PVP, and ethylene glycol purchased from Sigma Chemicals (St. Louis, MO, USA) were used without further purification. Separate solutions of 0.1 mol/L (AgNO3) and 0.6 mol/L (PVP) were prepared in anhydrous ethylene glycol. Each solution was stirred to complete the dissolution in a dry box under nitrogen atmosphere. Then, they were transferred into a Teflon vessel of 23 mL capacity microwave transparent body autoclave. The reactor was kept closed inside the dry box that was placed inside a conventional oven under a regulated power of 200 to 1,000 W. In order to prevent overpressure inside the reactor, the synthesis process was carried out by power pulses of 1.0 min and relaxation pulses of 0.5 min. The first relaxation pulse was for 0.5 min followed by a 1.0-min pulse. The reaction time to the total time of pulses with power for each treatment was between 5.0 and10 min. At the end of the reaction, the reactor was cooled down to room temperature. Cotton-like appearance was formed at the top of the reactor chamber; this was carefully removed with a spatula and was washed with deionized water and ethanol several times to remove the excess PVP from the Ag-NWs surface. The resulting material was rich in Ag-NWs of size approximately 70 to 110 nm. The residue left at the bottom of the reactor (approximately 5%) was discarded. Reactor power, reactor fill capacity, and molar ratio (PVP: AgNO3) were the parameters carefully considered in the synthesis.
Scanning transmission electron microscopy (STEM) was performed in a probe-corrected JEOL-JEM-ARM 200 F (JEOL Ltd., Akishima-shi, Japan) operated at 200 kV (point resolution of 0.08 nm). Scanning electron microscopy (SEM) was performed using a FEG Hitachi S-5500 ultra high-resolution scanning electron microscope (0.4 nm at 30 kV; Hitachi Ltd., Chiyoda-ku, Japan) with a BF/DF Duo-STEM detector.
Results and discussion
Experiments using both higher reactor power (1,200 W) and reactor fill capacity (40%) were also performed and is also shown in Figure 2a,b,c,d,e,f. Figure 2a,d and b,e corresponds to experiments carried out with different reaction times at 5 and 10 min, respectively. In the micrographs, it can be observed that a considerable increase, the reactor power leads to Ag-NWs of more than 30 μm in length and diameters ranging between 90 and 150 nm. Most of the NWs were found to intertwine forming agglomerates, as seen in Figure 2b,d. These structures were different from those obtained for 600 W. Ag-NWs synthesized with this reactor power were not found to intertwine or agglomerate but had smaller diameter. An increase in the pressure due to overheating of solvent was produced for 1,200 W. This reactor power produced Ag-NWs well before 5 min. Therefore, by raising reaction time, the Ag-NWs continue to grow until the ions in the solution gets depleted. Owing to high pressure in the reaction chamber, they begin to degrade leading to intertwines and agglomeration, as seen in Figure 2b,d. Increasing reactor power is counterproductive to obtain well-shaped and homogeneous silver nanowires. Characteristic picks of Ag metal appearing in the spectrum at 2,984 KeV [Ag(Lα)] and 3.151 KeV [Ag (Lβ)] observed in EDX analysis (Figure 2f) reveals that the NWs composition consists only of silver atoms.
To prevent degradation and intertwining of Ag-NWs as in previous cases, synthesis was performed at 800 W using two reactors fill capacity of 40% and 20%. Results obtained are shown in Figures 3 and 4, respectively. High production of Ag-NWs at 40% reactor fill capacity was observed because a possible explanation is that Ag2+ ions get reduced during the synthesis. NWs are then separated by decantation of the reaction solution. Ag-NPs get dispersed in the supernatant solution. After washing and drying under reduced pressure, a greater yield of 85% was obtained (Figure 3c,d). These NWs were above 50 μm and diameters ranging between 70 to 110 nm. They were not found to be intertwined as those obtained at 1,200 W (Figure 2b,d). Reaction time (5 min) was found to be ideal for appropriate preferential growth; in these experiments, it was observed that an excessive reaction time and reactor power are counterproductive in Ag-NWs synthesis. In order to optimize solvent suitable to produce an appropriate saturation pressure to achieve better performance and homogeneity of the NWs, it is important to try different reaction times and reactor powers. The reactor fill capacity in combination with the reactor power also affects the NWs dimensions, as these parameters are directly related to the system pressure. Figure 4 shows Ag-NWs obtained for 800 W and 20% of reactor fill capacity. These NWs were found to have smaller diameters than those obtained for 40% of reactor fill capacity, shown in Figure 3. Production declines on obtaining higher proportion of nanowires and nanoparticles mixture. In the MAH as well as in the conventional heating method, the following is evident: if one wishes to increase the yield percent of nanowires, the synthesis parameters must be increased. This leads to obtain nanomaterials larger in diameter and length. Conversely, a reduction in the parameters leads to lower dimensions and also low production. This is mainly owing to the system pressure which is very sensitive to the changes in the reactor power, reactor fill capacity, precursor's concentrations, and products formed in the reaction.
One of the major problems that arise in the application development of nanomaterials is controlling the size and shape of the nanostructures which, due to any temperature gradient, may lead to obtain a mixture of shapes and sizes of these. Another problem that arises is the amount of synthetic material. For that reason, with MAH method, it is possible to obtain silver nanowires fast and with high yield percentage. These materials can be used in the manufacture of optoelectronic devices; also, due to its surface plasmon resonance effect (SPR) , these can be used in the molecule detection and the manufacture of specific biosensors , isotropic conductive adhesives, solar cells, displays, touch panels, and organic light-emitting diodes, on-chip interconnects, and other typical applications of 1D nanostructured materials [37,38].
High yield of Ag-NWs were obtained by the MAH method. NWs diameter synthesized through this method ranged from 70 to 110 nm in diameter. Percentage rate of NWs depended largely on the synthesis parameters, especially, reactor power and reactor fill capacity. Higher yield of Ag-NWs was achieved at 800 W, 5 min of reaction time, and with 40% of reactor fill capacity. It was found that an excessive reactor power considerably deformed nanowires and produces large diameter and a lot of agglomerates of NWs, making the separation and purification process harder. In comparison to conventional hydrothermal method to produce Ag-NWs, MAH method produces nanowires of diameter greater than 50 nm; moreover, its productivity rate is also high.
The authors MFM would like to thank FONDECYT PROJECT No. 11110347 (Initiation into research Funding Competition) for financial support of this work, Government of Chile. CM, for the National Commission for Scientific and Technological Research, CONICYT No. 21110094 - Ministry of Education, Government of Chile for a PhD. Also the authors are grateful to electronic microscopy laboratory of the International Center for Nanotechnology and Advanced Materials at the University of Texas in San Antonio, USA. The Advanced Nanocomposites Research Group (GINA) at the Materials Engineering Department (DIMAT), University of Concepcion, Concepcion - Chile. Thanks to Yanet Estefany Macias Anguiano for her contributions to this work.
- Clayton DA, Benoist DM, Zhu Y, Pan SL. Photoluminescence and spectroelectrochemistry of single Ag nanowires. ACS Nano. 2010;4:2363–73.View ArticleGoogle Scholar
- Hu XH, Chan CT. Photonic crystals with silver nanowires as a near-infrared superlens. Appl Phys Lett. 2004;85:1520–2.View ArticleGoogle Scholar
- Zhang L, Wang B, Zhu G, Zhou X. Synthesis of silver nanowires as a SERS substrate for the detection of pesticide thiram. Spectrochim Acta A. 2014;133:411–6.View ArticleGoogle Scholar
- Wu HP, Liu JF, Wu XJ, Ge MY, Wang YW, Zhang GQ, et al. High conductivity of isotropic conductive adhesives filled with silver nanowires. Int J Adhes Adhes. 2006;26:617–21.View ArticleGoogle Scholar
- Baranova LA, Baryshev SV, Gusinskii GM, Konnikov SG, Nashchekin AV. Nickel field-emission microcathode: art of fabrication, properties, and applications. Nucl Instrum Meth B. 2010;268:1686–8.View ArticleGoogle Scholar
- Yin AJ, Li J, Jian W, Bennett AJ, Xu JM. Fabrication of highly ordered metallic nanowire arrays by electrodeposition. Appl Phys Lett. 2001;79:1039–41.View ArticleGoogle Scholar
- Aravamudhan S, Kumar A, Mohapatra S, Bhansali S. Sensitive estimation of total cholesterol in blood using Au nanowires based microfluidic platform. Biosens Bioelectron. 2007;22:2289–94.View ArticleGoogle Scholar
- Kumar A, Zhou C. The race to replace tin-doped indium oxide: which material will win? ACS Nano. 2010;4:11–4.View ArticleGoogle Scholar
- Chaney SB, Shanmukh S, Dluhy RA, Zhao YP. Aligned silver nanorods arrays produce high sensitivity surface-enhanced Raman spectroscopy substrates. Appl Phys Lett. 2005;87:031908–10.View ArticleGoogle Scholar
- Kondo Y, Takayanagi K. Gold nanobridge stabilized by surface structure. Phys Rev Lett. 1997;79:3455–8.View ArticleGoogle Scholar
- Kramer N, Birk H, Jorritsma J, Schonenberger C. Fabrication of metallic nanowires with a scanning tunneling microscope. Appl Phys Lett. 1995;66:1325–7.View ArticleGoogle Scholar
- Silvis-Cividjian N, Hagen CW, Kruit P, Stam MAJ, Groen HB. Direct fabrication of nanowires in an electron microscope. Appl Phys Lett. 2003;82:3514–6.View ArticleGoogle Scholar
- Chen CL, Furusho H, Mori H. Silver nanowires with a monoclinic structure fabricated by a thermal evaporation method. Nanotechnology. 2009;20:405605–9.View ArticleGoogle Scholar
- Liang C, Terabe K, Hasegawa T, Masakazu A. Resistance switching of an individual Ag2S/Ag nanowire heterostructure. Nanotechnology. 2007;18:485202–7.View ArticleGoogle Scholar
- Mohanty P, Yoon I, Kang T, Seo K, Varadwaj KSK, Choi W, et al. Simple vapor-phase synthesis of single-crystalline Ag nanowires and single-nanowire surface-enhanced Raman scattering. J Am Chem Soc. 2007;129:9576–7.View ArticleGoogle Scholar
- Eisele DM, Berlepsch HV, Bottcher C, Stevenson KJ, VandenBout DA, Kirstein S. Photoinitiated growth of sub-7 nm silver nanowires with in a chemically active organic nanotubular template. J Am Chem Soc. 2010;132:2104–5.View ArticleGoogle Scholar
- Zhao WB, Zhu JJ, Chen HY. Photochemical synthesis of Au and Ag nanowires on a porous aluminum oxide template. J Cryst Growth. 2003;258:176–80.View ArticleGoogle Scholar
- Fang J, Hahn H, Krupke R, Schramm F, Scherer T, Ding B. Silver nanowires growth via branch fragmentation of electrochemically grown silver dendrites. Chem Commun. 2009;9:1130–2.View ArticleGoogle Scholar
- Lin SC, Chen SY, Chen YT, Cheng SY. Electrochemical fabrication and magnetic properties of highly ordered silver–nickel core-shell nanowires. J Alloy Compd. 2008;449:232–6.View ArticleGoogle Scholar
- Peppler K, Janek J. Template assisted solid-state electrochemical growth of silver micro and nanowires. Electrochim Acta. 2007;53:319–23.View ArticleGoogle Scholar
- Huang X, Dong W, Ge Wang M, Yang LT, Feng Y, Zhang X. Synthesis of confined Ag nanowires within mesoporous silica via double solvent technique and their catalytic properties. J Colloid Interf Sci. 2011;359:40–6.View ArticleGoogle Scholar
- Xia YN, Yang PD, Sun YG, Wu YY, Mayers B, Gates B, et al. Templated surface sol–gel synthesis of SiO2 nanotubes and SiO2-insulated metal nanowires. Adv Mater. 2003;15:353–89.View ArticleGoogle Scholar
- Sun YG, Mayers B, Herricks T, Xia YN. Polyol synthesis of uniform silver nanowires: a plausible growth mechanism and the supporting evidence. Nano Lett. 2003;3:955–60.View ArticleGoogle Scholar
- Cleveland CL, Landman U. The energetics and structure of nickel clusters: size dependence. J Chem Phys. 1991;94:7376–96.View ArticleGoogle Scholar
- Wiley B, Herricks T, Sun Y, Xia Y. Polyol synthesis of platinum nanoparticles: control of morphology with sodium nitrate. Nano Lett. 2004;4:1733–9.View ArticleGoogle Scholar
- Wiley B, Sun Y, Xia Y. Polyol synthesis of silver nanostructures: control of product morphology with Fe(II) or Fe(III) species. Langmuir. 2005;21:8077–80.View ArticleGoogle Scholar
- Tang S, Vongehr S, Wan N, Meng X. Rapid synthesis of pentagonal silver nanowires with diameter-dependent tensile yield strength. Mater Chem Phys. 2013;142:17–26.View ArticleGoogle Scholar
- Zhang Y, Wang J, Yang P. Convenient synthesis of Ag nanowires with tunable length and morphology. Mater Res Bull. 2013;48:461–8.View ArticleGoogle Scholar
- Wiley B, Sun Y, Xia Y. Synthesis of silver nanostructures with controlled shapes and properties. Acc Chem Res. 2007;40:1067–76.View ArticleGoogle Scholar
- Guh-HwanLim SJ, Lee IH, Bok S, Lee JH, Nam J, Cho JH, et al. Polyolsynthesis of silver nanostructures: inducing the growth of nanowires by a heat-up process. Chem Phys Lett. 2014;602:10–5.View ArticleGoogle Scholar
- Jia C, Yang P, Zhang A. Glycerol and ethyleneglycol co-mediated synthesis of uniform multiple crystalline silver nanowires. Mater Chem Phys. 2014;143:794–800.View ArticleGoogle Scholar
- Reyes-Gasga J, Elechiguerra JL, Liu C, Camacho-Bragado A, Montejano-Carrizales JM, Jose YM. On the structure of nanorods and nanowires with pentagonal cross-sections. J Cryst Growth. 2006;286:162–72.View ArticleGoogle Scholar
- Tetsumoto T, Gotoh Y, Ishiwatari T. Mechanistic studies on the formation of silver nanowires by a hydrothermal method. J Colloid Interf Sci. 2011;362:267–73.View ArticleGoogle Scholar
- Im SH, Lee YT, Wiley B, Xia YN. Large-scale synthesis of silver nanocubes: the role of HCl in promoting cube perfection and monodispersity. Angew Chem Int. 2005;44:2154–7.View ArticleGoogle Scholar
- Olson TY, Zhang JZ. Structural and optical properties and emerging applications of metal nanomaterials. J Mater Sci Technol. 2008;4:433–46.Google Scholar
- Fang X, Hu L, Ye C, Zhang L. One-dimensional inorganic semiconductor nanostructures: a new carrier for nanosensors. Pure Appl Chem. 2010;82:2185–98.View ArticleGoogle Scholar
- Fang XS, Ye CH, LD Zhang JXZ, Zhao JW, Yan P. Direct observation of the growth process of MgO nanoflowers by a simple chemical route. Small. 2005;1:422–8.View ArticleGoogle Scholar
- Kim B-S, Lee S, Kim W-K, Park J-H, Cho YC, Kim J, et al. Fabrication of ZnCoO nanowires and characterization of their magnetic properties. Nanoscale Res Lett. 2014;9:221–7.View ArticleGoogle Scholar
This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/4.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly credited.